Journal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios


 Elaine Hall
 1 years ago
 Views:
Transcription
1 Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List of Authors: Muttashar, Majid; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Karunasena, Warna; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Manalo, Allan; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Lokuge, Weena; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Keywords: Abstract: Pultruded sections, fibre composites, elastic properties, characterization, shear span, fullscale testing It is important to determine accurately the elastic properties of fibre reinforced polymer (FRP) composites material, considering that their member design is often governed by deflection rather than strength. In this study, the elastic properties of the pultruded glass FRP (GFRP) square sections were evaluated firstly using fullscale with different shear span to depth (a/d) ratios and tested under static fourpoint bending. Back calculation and simultaneous methods were then employed to evaluate the flexural modulus and shear stiffness and were compared with the results of the coupon tests. Secondly, the fullscale beams were tested up to failure to determine their capacity and failure mechanisms. Finally, prediction equations describing the behaviour of the pultruded GFRP square beams were proposed and compared with the experimental results. The results indicate that the back calculation method gives more reliable values of elastic properties of GFRP profiles. In addition, the behaviour of the beams is strongly affected by the a/d ratios. The shear was found to have a significant contribution on the behaviour of beams with lower a/d ratios while the flexural stress played a major part for higher a/d ratios. The proposed equation, which accounts for the combined effect of the shear and flexural stresses, reasonably predicted the failure load of pultruded GFRP square beams.
2 Page of
3 Page of Research paper Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios (Title contains words) Running headline: Behaviour of Hollow Pultruded GFRP square Beams with Different Shear SpantoDepth Ratios ( characters) by Majid Muttashar,, Warna Karunasena, Allan Manalo,* and Weena Lokuge Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia Department of Civil Engineering, College of Engineering, University of Thi Qar, Iraq. Submitted to Corresponding Author * : Allan Manalo Senior Lecturer in Civil Engineering (Structural) Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, Queensland 0, Australia Manuscript summary: Total pages (including page cover) Number of figures Number of tables 0
4 Page of Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Abstract Majid Muttashar,, Warna Karunasena, Allan Manalo,* and Weena Lokuge It is important to determine accurately the elastic properties of fibre reinforced polymer (FRP) composites material, considering that their member design is often governed by deflection rather than strength. In this study, the elastic properties of the pultruded glass FRP (GFRP) square sections were evaluated firstly using fullscale with different shear span to depth (a/d) ratios and tested under static fourpoint bending. Back calculation and simultaneous methods were then employed to evaluate the flexural modulus and shear stiffness and were compared with the results of the coupon tests. Secondly, the fullscale beams were tested up to failure to determine their capacity and failure mechanisms. Finally, prediction equations describing the behaviour of the pultruded GFRP square beams were proposed and compared with the experimental results. The results indicate that the back calculation method gives more reliable values of elastic properties of GFRP profiles. In addition, the behaviour of the beams is strongly affected by the a/d ratios. The shear was found to have a significant contribution on the behaviour of beams with lower a/d ratios while the flexural stress played a major part for higher a/d ratios. The proposed equation, which accounts for the combined effect of the shear and flexural stresses, reasonably predicted the failure load of pultruded GFRP square beams. Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia Department of Civil Engineering, College of Engineering, University of Thi Qar, Iraq. * Corresponding author: Allan Manalo, Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia
5 Page of Keywords: Elastic properties, characterization, shear, flexural, failure load, GFRP beams Introduction Fibre reinforced polymer (FRP) composites emerged as a promising material to satisfy the increasing demand for better performing and more durable civil infrastructures. Recently, FRP composites have been used in bridges, because of their high stiffness, strengthtoweight ratios, corrosion resistance and durability. In addition to these superior properties, the process of producing FRP sections allows the designer to specify different material properties for different parts of the cross section. Nevertheless, the use of these advanced materials in structural applications is constrained due to limited knowledge on their material properties and structural behaviour. Therefore it is of paramount importance to investigate the properties of pultruded FRP sections so that they can be broadly utilised in structural applications. A number of micromechanical simulations have already been developed to predict the properties of pultruded beams such as flexural and shear modulus . The mechanical properties estimated using these models showed a good correlation with the experimental results. However, the models require accurate information on the processing details of the FRP profiles such as individual properties of fibres and resin, the fibre volume fraction and the composition of the laminates. Therefore, the use of these models as a design tool for structural purposes is likely to complicate the process. Thus, several researchers investigated coupon specimens to determine the effective mechanical properties of the composites and used these properties to predict the behaviour of full scale pultruded FRP profiles,. Manaloet al. 0 mentioned that there are limited test methods and equipment to characterise the properties of thick FRP composites by using the results of coupon tests. Moreover, the limited dimensions in the transverse direction of the majority of the pultruded GFRP sections added a new obstacle to the applicability of available test standards. The complex internal
6 Page of structure of composites and/or the variation of its mechanical properties within the element itself warrant testing of full scale sections to obtain realistic design properties. Guadeset al. conducted an experimental investigation to characterise the mechanical properties of square pultruded sections (00 mm x 00 mm) using both coupon and full scale specimens. Although, there was a good agreement between the coupon and fullscale results for single span beams, the effect of shear deformation on the behaviour of the pultruded profiles was neglected as the beam considered in sufficiently long. Bank indicated that the effect of shear on thin walled FRP sections is very significant especially for shorter beams and should be considered in determining the elastic properties of composite material. In support of this, Bank and Neto and Rovere conducted experiments using fullscale sections to determine the flexural (E) and shear (G) modulus of FRP composite beams. In both situations, three point bending tests were used to characterise the behaviour of beams with different spans. Even though same test procedure and almost similar section properties were used in both research, there was a huge difference between the calculated E/G ratios as Bank determined the elastic modulus based on Timoshenko Beam Theory while Neto and Rovere used the graphical (simultaneous) test method. Mottram stated that the sensitivity of the graphical method in determining the slope (of the regression line through the data points) can lead to a significant change in the E and G calculations. As a result, there is a need to revisit the graphical method used to find the flexural and shear modulus. To the authors knowledge, there are very limited experimental studies conducted to determine the structural properties of full scale FRP composite beams made of vinyl ester resin with Eglass fibre reinforcement oriented in different directions. In this study, hollow pultruded GFRP square beams with different shear spantodepth (a/d) ratios were tested using static four point bending configuration. Graphical (simultaneous) and back
7 Page of calculation methods were used to calculate the E and G and compared with the results of the coupon test. In addition, the effect of a/d ratio on the strength and failure behaviour of the GFRP beams was analysed. Based on the experimental results of this research, a simplified prediction equation to obtain the failure load of the GFRP beams was proposed with due consideration given to the effect of a/d ratio. These predicted failure loads are then compared with the experimental results. Determination of flexural and shear modulus (Beam Theory) The relatively low elastic modulus of GFRP leads to designs being governed by deflection and buckling limitations, instead of strength,. In addition, the anisotropic nature of the FRP composites results in low shear modulus to longitudinal elastic modulus ratio. Accordingly, the contribution of shear deformation in the total deformation becomes significant and should be considered in designing composite structures,,. This shear contribution can be theorised by using Timoshenko beam theory. This theory incorporates shear deformation of thin walled composite sections in deflection and investigates its effect in a quantitative manner in order to reliably determine the E and G for the pultruded FRP section. In this method the controlling equations are: = () + = where I is the second moment of area, is the bending slope, M is the bending moment, δ is the total deflection, V is the shear force and A is the cross sectional area. The shear coefficient K is a constant which accounts for the shear distribution over the beam cross section. For homogenous box profile, K can be calculated using the equation recommended by Bank : K= () ()
8 Page of where υ, G and E refer to the longitudinal Poisson s ratio, shear modulus and elastic modulus, respectively of the section. By solving equations and for the case of four point load bending with the load applied at a distance (a) from the support point (a=l/ in this case, where L is the beam span), the total deflection can be obtained as follows: = + where P is the total applied load, EI is the flexural stiffness and KGA is the shear stiffness. Two techniques are commonly used to calculate EI and KGA by using the above equation. The first technique is called back calculation method (BCM) which was based on the Bernoulli equation to determine the EI from the strain readings on the outer flange surfaces at midspan (in the constant moment region): = where c is the distance from the neutral axis to the outermost fibre, and ε is the measured strain. After EI is calculated, Equation can be used to back calculate KGA. The second technique is referred to as simultaneous method (SM) where at least two different spans should be investigated experimentally. Each test produces a data set for load, deflection and span. These three terms are known in Equation with EI and KGA as two unknowns. For better interpretation of the method, Equation is divided throughout by PL/A as follows: = + This represents a straight line, with (L/r) being the independent variable on the horizontal axis and Aδ/PL being the dependent variable on the vertical axis. Herein, r is the radius of gyration of the section defined by =. By plotting the variable () () () against, the elastic modulus can be found from the slope of the straight line and the shear modulus from the intercept on the vertical axis:
9 Page of = = Experiment program Material properties Pultruded GFRP square sections ( mm x mm x. mm thickness) produced by Wagner s Composite Fibre Technologies (WCFT), Australia were used in this study. These sections are made from vinyl ester resin with Eglass fibre reinforcement. The density of these pultruded profiles is 0 kg/m. As per standard ISO, the burnout test revealed an overall glass content of % by weight in these profiles. The stacking sequence of the plies is [0 0 /+ 0 /0 0 / 0 /0 0 / 0 /0 0 /+ 0 /0 0 ], where the 0 o direction aligns with the longitudinal axis of the tube. Table shows the mechanical properties of the pultruded sections determined from coupon tests. Table. Mechanical properties from coupon test Characterization of elastic properties for pultruded sections Following the methodology proposed by Bank, GFRP pultruded profiles with three different a/d ratios were tested under static four  point bending. The details of the tested specimens are listed in Table. The load was applied at the third points of the span and shear span to total length (a/l) was maintained at / for all tests. Figure shows the schematic illustration of the test setup and the tests were conducted according to ASTM D. A 00 kn capacity servo hydraulic testing machine was used with a loading rate of mm/min. All specimens were tested only up to approximately % of the failure load to ensure that the beams are still in the elastic range. Strain gauges (PFLL0) of mm length were attached to the bottom face at the midspan of the specimens. Laser displacement transducer () ()
10 Page of was used to measure the midspan deflection. The applied load and the deflection of the loading ram were recorded using the Systems 000 data acquisition system. Table. Details of the specimens tested for the elastic properties Figure. Experimental setup for characterisation of elastic properties. Behaviour of hollow pultruded GFRP composite beams Hollow GFRP pultruded sections with four different a/d ratios were tested up to failure under static four point bending test. In contrast to section., the load was applied at the two points with a load span equal to 00 mm. The constant load span was used to keep the upper face of the section under same condition for all specimens and to take account of the limitation on the length of the test frame. Vertical supports were provided to prevent lateral buckling. The details of the tested specimens are listed in Table. Figure shows the experimental set up. A 00 kn capacity universal machine was used for applying the load. Steel plates were provided at the support and loading points to minimise indentation failure. Table. Details of the specimens tested for the behaviour of GFRP beams Figure. Experimental setup for the behaviour of GFRP beams. Experimental results and observations The experimental results for the elastic properties and the behaviour of full scale beams are discussed in this section. Elastic properties of GFRP sections E and G using back calculation method. The load versus deflection curves for all specimens are shown in Figure. Linear elastic behaviour up to kn can be observed from these. The variations of E and KGA with load for all specimens are shown in Figures to. From these curves, it can be seen that these parameters start at a high value but reduce with increasing load. In order to minimise the errors that might have occurred due to deflection
11 Page 0 of measurements in this study, EI and KGA were computed from the average of several points spaced within a range of L/00 to L/00 deflection as suggested by Hayes and Lesko. The average calculated values of E and KGA from the BCM are summarized in Table. In this table, a numerical value for the moment of inertia has been used. The shear modulus G is separated from KGA using the k determined from equation () and the nominal cross section area of the beam. The average value of E was. GPa which is % higher than the coupon test results. The higher flexural modulus obtained from the full section compared with the coupon specimens can be related to the continuity of ± o fibres along the length of the pultruded beams. In addition, the shear modulus value of GPa is comparable with the value suggested by Mottram for a standard GFRP pultruded profile. Figure. Load deflection relationship for GFRP beams. Figure. Elastic modulus (E) and Shear stiffness (KGA) versus Load for a/d =. Figure. Flexural Modulus (E) and Shear Stiffness (KGA) versus Load for a/d =. Figure. Flexural Modulus (E) and Shear Stiffness (KGA) versus Load for a/d =. Table. Summary of average E and KGA for each span for GFRP beam testing (BCM) E and G using simultaneous method. In order to determine the elastic properties E and G, a graph for Aδ/PL versus (L/r) was plotted as shown in Figure. A linear regression was used to obtain the slope, intercept and the coefficient of correlation, which are also shown in the figure. The E and G values were then calculated using equations and, respectively. The calculated E in this method is. GPa which is higher than the coupon test results by about %. In contrast, G is. GPa which is less than the average value for standard pultruded profiles by about %. Figure. Typical graph to determine E and KG using simultaneous method. Behaviour of hollow pultruded GFRP composite beams
12 Page of Loaddeflection behaviour. Figure shows the load  deflection curves for the GFRP pultruded beams, which shows a linear behaviour until failure. There is a non linear response before the final failure for the beams with a/d ratios of. and.. This behaviour is possibly due to the crushing of the corners of the specimen at the support and at the loading points which leads to separation of the web flange junction. This progressive failure results in the web to continue carrying the applied load. The load carrying capacity of the beam is affected by the variation of the a/d ratio whereas a decreasing trend was observed with increasing a/d ratio. All the beams show a brittle failure in both flexural and transverse shear failure modes. Table presents a summary of the test results with respect to failure load, corresponding deflection and failure mode. Table. Summary of experimental results for GFRP beams Stress strain behaviour. The strain measurements for the beams at the top and bottom faces in addition to the strain at the shear path are shown in Figures to. It can be seen that the tension strain at the bottom face is higher than the top face compression strain (i.e. for a/d ratio of and stress MPa the tension strain reaches 00 micro strain compared with 000 microstrain in the compression side). There was a different trend in the strain on the top and bottom sides. The tension strains increased linearly up to failure, whereas the compression strains began to decrease non linearly as the load exceeded approximately % of the ultimate failure load. At the top side, the strain was negative demonstrating that the profile is compressed, as expected. With increasing load, however, the values tend to become positive indicating that the top surface is moving from being compressed to tensioned as shown in Figure. This behaviour reflects the onset of buckling considering that the flange can be assumed to be simply supported at the loading points. Consequently, the increase in the applied load increased the compression component of the moment which results in a local buckling of the flange. Figure 0 shows that the tensile strain decreases
13 Page of with decreasing shear span. The bottom side of the tested specimens were subjected to extensive tensile straining although failure cannot be observed there even after the compression region at the loading zone has failed entirely. Figure shows that shear strain increases with decreasing a/d due to the fact that a significant portion of the shear is transferred directly to the support by an inclined strut. As a result the amount of the direct load transfer increases with decreasing a/d ratio. In summary, the failure initiated at web flange junction and followed by buckling and/or crushing in the web depending on the a/d ratio: beams with higher a/d ratio experienced buckling failure whereas beams with lower a/d ratio experienced crushing. Figure. Load deflection curves for GFRP beams. Figure. Stress versus compression strain. Figure 0. Stress versus tensile strain. Figure. Stress versus shear strain. Failure mode. The different failure modes of the GFRP beams are shown in Figure. The observed failure modes can be classified as flexural failure and transverse shear failure. The shorter beams (a/d ratios of. and.) displayed progressive damage accumulation, which is indicated by the drops in the load deflection curves, with the increasing of the applied load. It was observed that the specimens had cracked and some twisted away from the centre towards one side. The mode of failure observed was transverse shear failure resulting in the delamination and cracking of the fibre along the edges of the pultruded beam in addition to local buckling on the compression flange as shown in Figures (a) and (b). Moreover, it was observed that the failure initiated at webflange junctions and followed by premature buckling and crushing in the webs. This failure behaviour is described as a potential failure for pultruded GFRP sections under concentrated bearing load conditions. For beams with a/d ratios of. and, the failure occurred at the points of loading and distinct cracks 0
14 Page of developed on the top surface and side of the tubes. Furthermore, cracks developed at the intersection between the flange and the web due to the buckling, leading to separation between them. It was also observed that delamination crack happened at the compression surface and later progressed into the sides as a result of local buckling initiation as shown in Figure (c) and (d). Similar observation was reported by Guadeset al. and Kumaret al. in their investigations on the flexural behaviour of 00 and mm square pultruded FRP tubes. In their studies, however, they reported that the final failure of the specimen occurs mainly due to the effect of the local buckling of the thin wall which results in material delamination and cracking of the fibre along the edges of the beam under the point loads. Shear crack was not observed even for beams with the lowest a/d ratio. The possible reason for this is the presence of the ± o plies in addition to the main fibre on the tube which provides a stronger shear resistance along the transverse direction. Figure. Failure modes of GFRP beams for different shear span to depth ratios. Discussion Determination of elastic properties. Table gives a summary of the properties of the GFRP profiles based on the coupon and full scale tests. It can be seen from this table that there is a significant difference between the results determined from coupon and full scale tests. The main reason between the coupon and full scale results is the effect of discontinuity of the fibres (especially the + o ) in the small solid coupon of composite material. However, the continuity of the fibres in the fullscale beam results in higher effective elastic properties than the coupon specimens. Using these properties, the loaddeflection behaviour of the fullscale pultruded GFRP beams were calculated using equation and compared with the experimental results. Figure displays comparison between the experimental and the predicted deflection calculated by using Timoshenko Beam Theory (equation ). Elastic properties obtained from full scale test (using BCM and SM) and coupon test have been used to predict the deflection.
15 Page of It can be seen that the Timoshenko Beam Theory provides a good approximation for the curves determined by the experimental tests. It can also be observed from the figure that using the elastic properties from BCM to calculate the beam deflection showed a good correlation with the experimental results for all a/d ratios. In contrast, analytical results using SM underestimated the experimental results and using coupon test results overestimated the deflection as shown in Figure. SM generally is relatively sensitive to the accuracy of the E measurement. When the span is short and for the same applied load, the deflection is in minimal. This observation is similar with Roberts and AlUbaidi wherein they indicated that the measured elastic properties of Pultruded FRP Iprofile can change substantially depending on the sensitivity of the graphical method. Therefore, it can be concluded that the elastic properties (E and G) determined using the BCM can reliably predict the behaviour of full scale GFRP beams. Figure shows the relationship between the flexural and shear deflection percentage of total deflection as a function of a/d ratio. The flexural and shear deflection was calculated using the average value obtained in this study (E/G =.). It can be seen that the flexural deflection constitutes approximately 0% of the total deflection for a/d of.. In contrast, shear deflection was 0 % for the same a/d ratio. These observations reflect the significant contribution of shear deformation in the total deflection of beams with low shear span to depth ratio. From the figure it can also be observed that the percentage of shear deflection is less than 0% for a/d of 0 and a ratio of is required to decrease the shear deflection to less than %. Therefore, for composite beams with a/d equal or less than 0 the effect of shear deformation should be accounted in the total deflection calculation. Table. Summary of experimental properties for GFRP beams Figure. Comparison of theoretical and experimental deflection of beams with different a/d ratios.
16 Page of Figure. Contribution of flexural and shear deflection for beams with different a/d ratios. Effect of a/d ratio on shear stress. The effects of shear span to depth ratio on the shear stress of the GFRP beams were evaluated by calculating the shear stress experienced by the beams using equation : τ= where V is the shear force, Q is the first moment of area, I is the moment of inertia, and t is the wall thickness. The calculated values of shear stress at failure for different a/d ratios of the GFRP beams are shown in Figure. The results showed that the a/d ratio has a significant effect on the shear stress experienced by the pultruded GFRP beams. The reason is that the shorter span beams can be subjected to higher failure load which means higher shear force resulting in higher shear stress according to Equation. As a result, it can be seen that the shear stress increases with decreasing a/d ratio. Similar behaviour has been documented for composite sandwich beams and timber beams tested with different a/d ratios . The authors indicated that shorter beam is subjected to a higher shear stress compared with longer span beams. They also mentioned that due to the core weakness, the shorter beams failed due to shear. In this study, no shear cracks were observed on the tested beams at the region of maximum shear even for short span beams. The relationship between the shear stress and the a/d ratios seems to be linear. Almost all the tested sections failed in similar mode by local buckling under the applied load followed by cracking at the compression side and the delamination of the plies. Although the tensile strain is low for small a/d ratios, the bottom face of the beam displays a crushing of fibres at the support without any failure at the midspan as shown in Figure. The reason for this is the higher applied load corresponding to lower a/d ratio. ()
17 Page of The maximum calculated shear stress of the pultruded GFRP beams with shear span to depth ratio of. and are and MPa, respectively. These shear stresses are % and %, respectively, of the shear strength of the pultruded profile given in Table. These lower percentages indicated that the shear stress is not only the factor which affected the behaviour of the pultruded beams but also the flexural stress. Manaloet al. 0 mentioned that these combined stresses played an important part in understanding the overall behaviour of composites and should be considered in the design and analysis of composite materials. Figure. Shear stress versus shear span to depth ratio for GFRP beam. Effect of a/d ratio on flexural stress. The flexural behaviour of the GFRP hollow sections have been studied by calculating the bending stress using equation 0: σ= The calculated bending stresses for GFRP beams with different a/d ratios are shown in Figure. It can be seen that the bending stress increases with increasing a/d ratio. The maximum bending stress with a/d ratios of. and are and 00 MPa, respectively. These bending stress values are % and % of the compression strength, respectively, and % and %, respectively, of the tensile strength of the pultruded profile as mentioned in Table. This explains the reason why the failure is happening at the compression side. Furthermore, the results indicated that the specimen experiences considerable flexural stresses even at a/d ratio of. which contributed to the failure mechanisms. Similar result was reported by Turvey and Zhang in their investigation on the shear failure strength of web flange junctions in pultruded GRP profiles. In their study, however, they reported that failure is a function of (0) combined high shear and bending stresses at the interfaces of different plies. Figure. Bending stress versus shear span to depth ratio for GFRP beam.
18 Page of Effect of a/d ratio on failure mode. The GFRP pultruded beams showed a brittle failure mode. The failure happened without any reduction in the slope of the load deflection behaviour. The beams with a/d ratio of more than exhibited a flexural mode of failure. The failure of those beams was controlled by the buckling under the load points followed by cracks and delamination at the compression face in addition to a web flange junction failure as shown in Figures (c) and (d). The beams with a/d less than showed a transverse shear failure. This type of failure was resulting in the delamination and cracking of the fibre along the edges of the pultruded beam in addition to local buckling on the compression flange. This failure behaviour was reported by Turvey and Zhang and Wu and Bai as a web flange junction failure which caused mainly by the concentrated bearing load conditions. A change in the slope of the load deflection behaviour has been noticed. In some cases, it can be seen that there are some drops in the load at the failure progress stage for the beams with spans lower a/d ratios. This failure response is due to the progressive damage accumulation of the section. No pure shear failure or shear cracks appeared in all of the tested beams. The main reason for that is the stacking sequence of the plies of the GFRP pultruded sections are in the form of ± degrees. It was clearly noticed that the failure cracks position was closer to the top loading point than to the supports. Prediction of failure load for pultruded GFRP beams with different a/d ratio The contribution of the shear deformation was clearly observed for all a/d ratios considered in this study. Therefore, in order to estimate the failure load of the pultruded GFRP beams, it is important to account for the shear and the bending stresses in the prediction equation. Proposed prediction equation Based on the experimental results, buckling failure occurred at the concentrated load points and/or near the support locations. The main reason for this behaviour is the high shear forces
19 Page of that typically develop at those locations. Bank stated that, when the beam is subjected to high shear forces and high bending moment, the web is subjected to combined shear stress (τ) and axial compressive or tensile (flexural) stress,. As a result, the combined effect of both stresses is significant and should be accounted for in the prediction of failure load. Structural plastics design manual ASCE recommends using an interaction equation based on the isotropic plate theory to calculate the critical load which takes into account the combined effect of shear and flexural stresses. This equation expressed in the form: + () where and τ act are the actual flexural and shear stresses, respectively, and τ all are the corresponding material allowable stresses. In this formula the combined effect of the shear and flexure has been suggested and the failure load can be calculated using the following equation: = () In this study, a linear interaction equation similar to ASCE equation is proposed to predict the failure load of the pultruded GFRP beams which account for the combined effect of shear and flexure. In the proposed equation, buckling stress calculated according to Bank has been used instead of the allowable compressive strength due to the fact that almost all the tested hollow pultruded profiles failed with local buckling. Therefore, the predicted failure load of the pultruded GFRP beams can be calculated as: = () The allowable stresses of the pultruded GFRP material are listed in Table. Comparison between predicted and the experimental failure loads
20 Page of The predicted failure load of the pultruded GFRP beams tested using point load and the percentage difference between the predicted and actual (experimental) average failure loads are summarised in Table. For clarity, the comparison is also shown in Figure. It can be seen from Table and Figure that the proposed equation () shows a good agreement between the predicted and the actual failure load. For beam with a/d ratio., the proposed equation overestimates the failure load by %. This indicates that the beams are more likely to fail by transverse shear failure and the shear has the higher effect on the section s failure mode. In contrast, the flexural compression stress is the more dominant stress to cause the failure for pultruded beams with a/d ratios of.. Moreover, it can be clearly noticed that the use of equation () to predict the failure load depends on the ultimate flexural stress will overestimate the failure load by as much as to %. Figure shows the percentages of stress contribution from the failure stress of the pultruded beams. As seen from the figure, for beams of a/d ratio., shear stress contribution (%) for the failure load is higher than that for the flexural stress (%). For beams with higher a/d ratio, the flexural stress becomes the dominant stress to cause the failure with % of the failure load compared with % of shear stress, respectively. These percentages showed that the predicted contributions compare well with the experimental contributions for shear and flexural stresses. In general, the proposed equation provided a conservative but practical estimation of the failure load of the pultruded GFRP beams with different a/d ratios. Table. Predicted failure load compared with the actual failure load Figure. Comparison between the predicted and the actual failure loads. Figure. Percentages of stress contribution from the total failure stress. Conclusions
21 Page of The behaviour of GFRP pultruded square beams with different shear span to depth (a/d) ratios was investigated using the fourpoint bending test. Similarly, the elastic properties of the beams were determined by testing fullscale specimens. The following conclusions can be drawn based on the results of the investigation:. The back calculation method gives more reliable values of effective flexural and shear moduli of pultruded hollow GFRP square sections compared with simultaneous method and coupon test. This method is based on the Bernoulli equation and uses the strain readings at midspan of the beam. A good correlation between the predicted and the actual loaddeflection behaviour was achieved using the elastic properties determined from this method.. The shear deformation contributes by as much as 0% to the total deflection of beams with low a/d ratio. Thus, it is recommended to account for the shear deflection in the deflection calculation of GFRP beams when (a/d) is less than or equal to.. The shear stress experienced by the beam decreases with increasing a/d. In contrast, the flexural stress increases with increasing a/d ratio.. The failure of the beam is governed by the buckling under the loading points followed by cracks and delamination at the webflange junction at the compression face.. The proposed equation accounting for the combined effect of shear and flexural stresses in pultruded GFRP square beams and accounting for the buckling stress of composites reasonably predicted the failure load of full size pultruded GFRP beams.. Aside from shear and flexural stresses, it was found that there is a complexity on the overall behaviour of pultruded GFRP square beams with low a/d, which needs further investigation. Acknowledgement
22 Page of The authors would like to acknowledge the support of Wagner s Composite Fibre Technologies (WCFT) for providing the GFRP pultruded sections. The first author would like to acknowledge the financial support by the Ministry of Higher Education and Scientific ResearchIraq. References. Bakis C, Bank LC, Brown V, et al. Fiberreinforced polymer composites for constructionstateoftheart review. Journal of Composites for Construction. 0; : .. Hollaway L. A review of the present and future utilisation of FRP composites in the civil infrastructure with reference to their important inservice properties. Construction and Building Materials. 0; : .. Bank LC. Shear coefficients for thinwalled composite beams. Composite Structures. ; : .. Barbero EJ, Fu SH and Raftoyiannis I. Ultimate bending strength of composite beams. Journal of Materials in Civil Engineering. ; : 0.. Omidvar B. Shear coefficient in orthotropic thinwalled composite beams. Journal of Composites for Construction. ; : .. Nagaraj V and GangaRao HV. Static behavior of pultruded GFRP beams. Journal of Composites for Construction. ; : 0.. Bank LC. Composite for Construction Structural Design with FRP Materials. New Jersey: Jone Wiley & Sons, 0, p... Davalos JF, Salim H, Qiao P, LopezAnido R and Barbero E. Analysis and design of pultruded FRP shapes under bending. Composites Part B: Engineering. ; : 0.. Roberts T and Masri H. Section properties and buckling behavior of pultruded FRP profiles. Journal of reinforced plastics and composites. 0; : Manalo A, Mutsuyoshi H and Matsui T. Testing and characterization of thick hybrid fibre composites laminates. International Journal of Mechanical Sciences. ; : 0.. Cardoso D, Harries K and Batista E. On the Determination of Mechanical Properties for Pultruded GFRP Sections. International Conference on FRP composites in Civil Engineering. Vancouver, Canada: Internationl Institute for FRP in Construction.. Guades E, Aravinthan T and Islam MM. Characterisation of the mechanical properties of pultruded fibrereinforced polymer tube. Materials & Design. ; : 0.. Bank LC. Flexural and shear moduli of fullsection fiber reinforced plastic(frp) pultruded beams. Journal of Testing and Evaluation. ; : 0.. Neto A and Rovere H. Flexural stiffness characterization of fiber reinforced plastic (FRP) pultruded beams. Composite structures. 0; : .. Mottram J. Shear modulus of standard pultruded fiber reinforced plastic material. Journal of Composites for Construction. 0; : .. Chambers RE. ASCE design standard for pultruded fiberreinforcedplastic (FRP) structures. Journal of Composites for Construction. ; : .. Parke G and Hewson N. ICE manual of bridge engineering. history. 0; :.. ISO. Textileglassreinforced plastics, prepegs, moulding compounds and laminates: Determination of the textileglass and mineralfiller content Calcination methods... ASTM D. ASTM D/DM0 Standard practice for determine sandwich beam flexural and shear stiffeness. West Conshohocken, (PA): ASTM International, 0.. Hayes M and Lesko J. The effect of nonclassical behaviors on the measurement of the Timoshenko shear stiffness. Proc nd Inter Conf FRP Composites in Civil Engineering CICE. 0, p. 0.
23 Page of Wu C and Bai Y. Web crippling behaviour of pultruded glass fibre reinforced polymer sections. Composite Structures. ; 0: Kumar P, Chandrashekhara K and Nanni A. Structural performance of a FRP bridge deck. Construction and Building Materials. 0; : .. Roberts T and AlUbaidi H. Flexural and torsional properties of pultruded fiber reinforced plastic Iprofiles. Journal of Composites for Construction. 0; : .. Dai J and Hahn HT. Flexural behavior of sandwich beams fabricated by vacuumassisted resin transfer molding. Composite Structures. 0; : .. Yoshihara H and Furushima T. Shear strengths of wood measured by various short beam shear test methods. Wood science and technology. 0; : .. Awad ZK, Aravinthan T and Manalo A. Geometry effect on the behaviour of single and gluelaminated glass fibre reinforced polymer composite sandwich beams loaded in fourpoint bending. Materials & Design. ; : 0.. Turvey GJ and Zhang Y. Shear failure strength of web flange junctions in pultruded GRP WF profiles. Construction and Building Materials. 0; : .. ASCE. Structural Plastics Design Manual. ASCE Manuals and Reports on Engineering Practice. Reston, VA: American Society of Civil Engineering,.
24 Page of *All dimensions are in mm as per Table mm All Figures Figure. Experimental setup for characterisation of elastic properties P mm a 00 mm a L *All dimensions are in mm as per Table Figure. Experimental setup for the behaviour of GFRP beams Figure. Load deflection relationship for GFRP beams
25 Page of Figure. Elastic modulus (E) and shear stiffness (KGA) versus Load for a/d =. Figure. Flexural modulus (E) and shear stiffness (KGA) versus Load for a/d =. Figure. Flexural modulus (E) and shear stiffness (KGA) versus Load for a/d =.
26 Page of Figure. Typical graph to determine E and KG using SM Figure. Load deflection curves for GFRP beams Figure. Stress versus compression strain
27 Page of Figure 0. Stress versus tensile strain Figure. Stress versus shear strain
28 Page of (a) a/d=. (c) a/d=. (d) a/d= Figure. Failure modes of GFRP beams for different shear span to depth ratios Figure. Comparison of theoretical and experimental deflection of beams with different a/d ratios
29 Page of Figure. Contribution of flexural and shear deflection for beams with different a/d ratios Figure. Shear stress versus shear span to depth ratio for GFRP beam Figure. Bending stress versus shear span to depth ratio for GFRP beam
30 Page of Figure. Comparison between the predicted and the actual failure loads Figure. Percentages of stress contribution from the total failure stress
31 Page 0 of All Tables Table. Mechanical properties from coupon test Properties Average value SD Compressive modulus (Longitudinal), GPa. Compressive strength, MPa 0 Tensile modulus (Longitudinal), GPa Tensile Strength (MPa) Flexural modulus (Longitudinal) (GPa).. Shear modulus (Longitudinal) (GPa). 0. Shear Strength (MPa) 0 Interlaminar shear strength (MPa) Table. Details of the specimens tested for the elastic properties Span length mm Shear span, a mm a/d Table. Details of the specimens tested for the behaviour of GFRP beams Span length mm Shear span, a mm a/d Table. Summary of average E and KGA for each span for GFRP beam testing (BCM) a/d E GPa C.O.V % KGA GPacm C.O.V % G GPa Ave..
32 Page of Table. Summary of experimental results for GFRP beams Shear span/ depth Average failure load Deflection Failure mode kn mm. TS TS: transverse shear failure F: flexural failure. TS. 0. F 0. F Table. Summary of experimental properties for GFRP beams Test type E modulus GPa G modulus GPa Coupon.. BCM. SM.. Table. Predicted failure load compared with the actual failure load a/d ratio Exp. kn Eq. kn Eq. kn
FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationFinite Element Analysis of FRP Debonding Failure at the Tip of Flexural/Shear Crack in Concrete Beam
Marquette University epublications@marquette Civil and Environmental Engineering Faculty Research and Publications Civil and Environmental Engineering, Department of 1212013 Finite Element Analysis
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationDETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS. Abstract
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
More informationDynamic and buckling analysis of FRP portal frames using a lockingfree finite element
Fourth International Conference on FRP Composites in Civil Engineering (CICE8) 2224July 8, Zurich, Switzerland Dynamic and buckling analysis of FRP portal frames using a lockingfree finite element F.
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationManuscript Draft. Title: Testing and analysis of pultruded GFRP continuous beams for the deflection serviceability limit state
Structures Elsevier Editorial System(tm) for Composite Manuscript Draft Manuscript Number: COSTD1502074R1 Title: Testing and analysis of pultruded GFRP continuous beams for the deflection serviceability
More informationExperimental investigation on monotonic performance of steel curved knee braces for weldfree beamtocolumn connections
Experimental investigation on monotonic performance of steel curved knee braces for weldfree beamtocolumn connections *Zeyu Zhou 1) Bo Ye 2) and Yiyi Chen 3) 1), 2), 3) State Key Laboratory of Disaster
More informationAccordingly, the nominal section strength [resistance] for initiation of yielding is calculated by using Equation CC3.1.
C3 Flexural Members C3.1 Bending The nominal flexural strength [moment resistance], Mn, shall be the smallest of the values calculated for the limit states of yielding, lateraltorsional buckling and distortional
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationUNIT III DEFLECTION OF BEAMS 1. What are the methods for finding out the slope and deflection at a section? The important methods used for finding out the slope and deflection at a section in a loaded
More informationGEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE
GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.02225767328 email: cejnm@civil.iitb.ac.in Module13 LECTURE
More informationEngineering Science OUTCOME 1  TUTORIAL 4 COLUMNS
Unit 2: Unit code: QCF Level: Credit value: 15 Engineering Science L/601/10 OUTCOME 1  TUTORIAL COLUMNS 1. Be able to determine the behavioural characteristics of elements of static engineering systems
More informationStructural behaviour of GFRP beams subjected to concentrated loads: experimental tests, numerical modeling and analytical study
Structural behaviour of GFRP beams subjected to concentrated loads: experimental tests, numerical modeling and analytical study Lourenço Almeida Fernandes, IST/DE Civil Abstract: GFRP composites have shown
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationCHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS
CHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS S. YanesArmas, J. De Castro and T. Keller Composite Construction Laboratory (CCLab), Ecole Polytechique Fédérale
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationChapter 4. Test results and discussion. 4.1 Introduction to Experimental Results
Chapter 4 Test results and discussion This chapter presents a discussion of the results obtained from eighteen beam specimens tested at the Structural Technology Laboratory of the Technical University
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationREGRESSION MODELING FOR STRENGTH AND TOUGHNESS EVALUATION OF HYBRID FIBRE REINFORCED CONCRETE
REGRESSION MODELING FOR STRENGTH AND TOUGHNESS EVALUATION OF HYBRID FIBRE REINFORCED CONCRETE S. Eswari 1, P. N. Raghunath and S. Kothandaraman 1 1 Department of Civil Engineering, Pondicherry Engineering
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More informationCE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR
CE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR 20142015 UNIT  1 STRESS, STRAIN AND DEFORMATION OF SOLIDS PART A 1. Define tensile stress and tensile strain. The stress induced
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationCHARACTERIZING INFLUENCE OF LAMINATE CHARACTERISTICS ON ELASTIC PROPERTIES OF CROSS LAMINATED TIMBER
CHARACTERIZING INFLUENCE OF LAMINATE CHARACTERISTICS ON ELASTIC PROPERTIES OF CROSS LAMINATED TIMBER Jan Niederwestberg 1, Ying Hei Chui ABSTRACT: Properties of CLT panels are influenced by the properties
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationMODULE C: COMPRESSION MEMBERS
MODULE C: COMPRESSION MEMBERS This module of CIE 428 covers the following subjects Column theory Column design per AISC Effective length Torsional and flexuraltorsional buckling Builtup members READING:
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationModelling of delamination damage in composite beams. 1 Introduction. Manudha T. Herath 1*, Kaustav Bandyopadhyay 1 and Joshua D.
6 th Australasian Congress on Applied Mechanics, ACAM 6 1215 December 2010, Perth, Australia Modelling of delamination damage in composite beams Manudha T. Herath 1*, Kaustav Bandyopadhyay 1 and Joshua
More informationLecture04 Design of RC Members for Shear and Torsion
Lecture04 Design of RC Members for Shear and Torsion By: Prof. Dr. Qaisar Ali Civil Engineering Department UET Peshawar drqaisarali@uetpeshawar.edu.pk www.drqaisarali.com 1 Topics Addressed Design of
More informationLONGTERM STABILITY OF PULTRUDED GLASS FIBERREINFORCED POLYMER COLUMNS. Qi Guo. Bachelor of Engineering, Tongji University, 2015
LONGTERM STABILITY OF PULTRUDED GLASS FIBERREINFORCED POLYMER COLUMNS by Qi Guo Bachelor of Engineering, Tongji University, 2015 Submitted to the Graduate Faculty of Swanson School of Engineering in
More informationtwenty one concrete construction: shear & deflection ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture twenty one concrete construction: Copyright Kirk Martini shear & deflection Concrete Shear 1 Shear in Concrete
More informationDesign of Beams (Unit  8)
Design of Beams (Unit  8) Contents Introduction Beam types Lateral stability of beams Factors affecting lateral stability Behaviour of simple and built  up beams in bending (Without vertical stiffeners)
More informationPOSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS
POSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS  Technical Paper  Tidarut JIRAWATTANASOMKUL *1, Dawei ZHANG *2 and Tamon UEDA *3 ABSTRACT The objective of this study is to propose a new
More informationDETERMINATION OF DUCTILITY CAPACITY AND OTHER SECTION PROPERTIES OF TSHAPED RC WALLS IN DIRECT DISPLACEMENTBASED DESIGN
DETERMINATION OF DUCTILITY CAPACITY AND OTHER SECTION PROPERTIES OF TSHAPED RC WALLS IN DIRECT DISPLACEMENTBASED DESIGN E. Smyrou 1, T.J. Sullivan 2, M.J.N. Priestley 3 and G.M. Calvi 4 1 PhD Candidate,
More informationNumerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods.
Numerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods. Giuseppe Giambanco 1, Tiziana Turetta 1, Alessia Cottone 1 1 Department of Structural, Aerospace
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationDEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS
DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS Konstantinos CHRISTIDIS 1, Emmanouil VOUGIOUKAS 2 and Konstantinos TREZOS 3 ABSTRACT
More informationFLEXIBILITY METHOD FOR INDETERMINATE FRAMES
UNIT  I FLEXIBILITY METHOD FOR INDETERMINATE FRAMES 1. What is meant by indeterminate structures? Structures that do not satisfy the conditions of equilibrium are called indeterminate structure. These
More informationStructural Analysis Laboratory. Michael Storaker, Sam Davey and Rhys Witt. JEE 332 Structural Analysis. 4 June 2012.
Structural Analysis Laboratory Michael Storaker, Sam Davey and Rhys Witt JEE 332 Structural Analysis 4 June 2012 Lecturer/Tutor Shinsuke Matsuarbara 1 Contents Statically Indeterminate Structure Objective...
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationSabah Shawkat Cabinet of Structural Engineering Walls carrying vertical loads should be designed as columns. Basically walls are designed in
Sabah Shawkat Cabinet of Structural Engineering 17 3.6 Shear walls Walls carrying vertical loads should be designed as columns. Basically walls are designed in the same manner as columns, but there are
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationMINE ROOF SUPPORT DESIGN AND ANALYSIS. Document no : Revision no : 1.0
MINE ROOF SUPPORT DESIGN AND ANALYSIS Document no : 1806269723 Revision no : 1.0 DOCUMENT TITLE : MINE ROOF SUPPORT DESIGN AND ANALYSIS DOCUMENT NUMBER : 1806269723 ISSUE : Issue 1.0 DATE : 7 October
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationCIVIL DEPARTMENT MECHANICS OF STRUCTURES ASSIGNMENT NO 1. Brach: CE YEAR:
MECHANICS OF STRUCTURES ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes XX and YY of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine
More informationBEAMS AND PLATES ANALYSIS
BEAMS AND PLATES ANALYSIS Automotive body structure can be divided into two types: i. Frameworks constructed of beams ii. Panels Classical beam versus typical modern vehicle beam sections Assumptions:
More information2. (a) Explain different types of wing structures. (b) Explain the advantages and disadvantages of different materials used for aircraft
Code No: 07A62102 R07 Set No. 2 III B.Tech II Semester Regular/Supplementary Examinations,May 2010 Aerospace Vehicle Structures II Aeronautical Engineering Time: 3 hours Max Marks: 80 Answer any FIVE
More informationDownloaded from Downloaded from / 1
PURWANCHAL UNIVERSITY III SEMESTER FINAL EXAMINATION2002 LEVEL : B. E. (Civil) SUBJECT: BEG256CI, Strength of Material Full Marks: 80 TIME: 03:00 hrs Pass marks: 32 Candidates are required to give their
More informationME 354, MECHANICS OF MATERIALS LABORATORY COMPRESSION AND BUCKLING
ME 354, MECHANICS OF MATERIALS LABATY COMPRESSION AND BUCKLING PURPOSE 01 January 2000 / mgj The purpose of this exercise is to study the effects of end conditions, column length, and material properties
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationTemperature Effects on a Fibre Reinforced Polymer Material
University of Southern Queensland Faculty of Engineering and Surveying Temperature Effects on a Fibre Reinforced Polymer Material A dissertation submitted by Samuel David William Zerbst in fulfilment of
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationNational Exams May 2015
National Exams May 2015 04BS6: Mechanics of Materials 3 hours duration Notes: If doubt exists as to the interpretation of any question, the candidate is urged to submit with the answer paper a clear
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationNew fibrereinforced polymer box beam: investigation of static behaviour
New fibrereinforced polymer box beam: investigation of static behaviour by Mario Springolo BE (Civil) (Hons I) A dissertation submitted for the award of DOCTOR OF PHILOSOPHY Faculty of Engineering and
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationStress Analysis Lecture 4 ME 276 Spring Dr./ Ahmed Mohamed Nagib Elmekawy
Stress Analysis Lecture 4 ME 76 Spring 017018 Dr./ Ahmed Mohamed Nagib Elmekawy Shear and Moment Diagrams Beam Sign Convention The positive directions are as follows: The internal shear force causes a
More informationChapter Objectives. Design a beam to resist both bendingand shear loads
Chapter Objectives Design a beam to resist both bendingand shear loads A Bridge Deck under Bending Action Castellated Beams Posttensioned Concrete Beam Lateral Distortion of a Beam Due to Lateral Load
More informationStructural Steelwork Eurocodes Development of A Transnational Approach
Structural Steelwork Eurocodes Development of A Transnational Approach Course: Eurocode Module 7 : Worked Examples Lecture 0 : Simple braced frame Contents: 1. Simple Braced Frame 1.1 Characteristic Loads
More informationMoment redistribution of continuous composite Igirders with high strength steel
Moment redistribution of continuous composite Igirders with high strength steel * Hyun Sung Joo, 1) Jiho Moon, 2) IkHyun sung, 3) HakEun Lee 4) 1), 2), 4) School of Civil, Environmental and Architectural
More informationStress Analysis Lecture 3 ME 276 Spring Dr./ Ahmed Mohamed Nagib Elmekawy
Stress Analysis Lecture 3 ME 276 Spring 20172018 Dr./ Ahmed Mohamed Nagib Elmekawy Axial Stress 2 Beam under the action of two tensile forces 3 Beam under the action of two tensile forces 4 Shear Stress
More informationExperimental and Predicted Behavior of FRP BeamColumns Including Retrofitting
Old Dominion University ODU Digital Commons Civil & Environmental Engineering Theses & Dissertations Civil & Environmental Engineering Fall 2015 Experimental and Predicted Behavior of FRP BeamColumns
More informationR13. II B. Tech I Semester Regular Examinations, Jan MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) PARTA
SET  1 II B. Tech I Semester Regular Examinations, Jan  2015 MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) Time: 3 hours Max. Marks: 70 Note: 1. Question Paper consists of two parts (PartA and PartB)
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More information